Site Preference and Ordering Induced by Au Substitution in the γ-Brass Related Complex Au-Cr-Zn Phases
Partha Pratim Jana; Ryan Henderson; Bernd Harbrecht; Sven Lidin; Inorganic Chemistry 52 (2013) 4812–4818; doi:10.1021/ic302244e

data_4334556
_publ_contact_author_address
;
CAS Chemical Centre
P O B 124
221 00 Lund
Sweden
;
_publ_contact_author_email       Partha.Jana@polymat.lth.se
_publ_contact_author_name        'Patha Pratim Jana'
_publ_section_title
;
 Site Preference and Ordering Induced by Au Substitution in the \g-Brass
 Related Complex Au-Cr-Zn Phases
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4812
_journal_page_last               4818
_journal_paper_doi               10.1021/ic302244e
_journal_volume                  52
_journal_year                    2013
_chemical_formula_sum            'Au3.8 Cr5.32 Zn91.75'
_chemical_formula_weight         7022.15
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           216
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  'F -4 2 3'
_symmetry_space_group_name_H-M   'F -4 3 m'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2012-09-20 # Formatted by publCIF
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   18.325(2)
_cell_length_b                   18.325(2)
_cell_length_c                   18.325(2)
_cell_measurement_temperature    293(2)
_cell_volume                     6153.6(12)
_computing_cell_refinement       'IPDS software'
_computing_data_collection       'IPDS software'
_computing_data_reduction        'IPDS software/X-RED'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'direct methods/Shelxs-97'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  IPDS(Stoe&Cie.)
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1120
_diffrn_reflns_av_sigmaI/netI    0.0347
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       27
_diffrn_reflns_limit_k_min       -28
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            22811
_diffrn_reflns_theta_full        33.08
_diffrn_reflns_theta_max         33.08
_diffrn_reflns_theta_min         3.14
_exptl_absorpt_coefficient_mu    44.850
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-shape
_exptl_crystal_colour            'silvery with metallic luster'
_exptl_crystal_density_diffrn    7.580
_exptl_crystal_F_000             12720
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.06
_exptl_crystal_size_min          0.04
_refine_diff_density_max         2.728
_refine_diff_density_min         -2.308
_refine_diff_density_rms         0.509
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   -0.02(2)
_refine_ls_extinction_coef       0.00019(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.078
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     80
_refine_ls_number_reflns         1204
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.078
_refine_ls_R_factor_all          0.0557
_refine_ls_R_factor_gt           0.0515
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0884P)^2^+391.7215P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1339
_refine_ls_wR_factor_ref         0.1377
_reflns_number_gt                1108
_reflns_number_total             1204
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic302244e_si_001_06.cif
_cod_data_source_block           V
_cod_original_sg_symbol_Hall     'F -4;2;3'
_cod_original_formula_sum        'Au3.80 Cr5.32 Zn91.75'
_cod_database_code               4334556